tr-108705np, 'bwr vessel and internals project, technical ... report summary the boiling water...
Post on 25-Sep-2019
Embed Size (px)
BWR Vessel and Internals Project Technical Basis for Inspection Relief for BWR Internal Components with Hydrogen Injection (BWRVIP-62NP)
NON-PROPRIETARY INFORMATION NOTICE: This report contains the non-proprietary information that is included in
the proprietary version of this report. The proprietary version of this report contains proprietary information that is the intellectual property of BWRVIP utility members and EPRI. Accordingly, the proprietary report is available only under license from EPRI and may not be reproduced or disclosed, wholly or in part, by any Licensee to any other person or organization.
The Boiling Water Reactor Vessel and Internals Project (BWRVIP), formed in June 1994, is an association of utilities focused exclusively on BWR vessel and internals issues. This report provides a systematic methodology for evaluating the effectiveness of hydrogen water chemistry (HWC) for the mitigation of intergranular stress corrosion cracking (IGSCC) of reactor internals when direct measurements of the internals' corrosion potential is not feasible.
BWR availability has been negatively impacted by the IGSCC o austenitic stainless steel piping and, more recently, reactor internal components. As mandated by the Nuclear Regulatory Commission (NRC), regular inspection is necessary for BWR piping to provide adequate assurance of structural integrity of affected piping systems. Similar inspections may be required for reactor internal components. However, due to the difficulty and expense of reactor internals inspections, it is clearly desirable to demonstrate that fewer inspections are necessary when suitable reactor internals IGSCC mitigation steps are taken.
The HWC process has been developed along two parallel paths to provide reactor internals IGSCC mitigation. The first internals IGSCC mitigation technique, moderate HWC (HWC-M), involves higher hydrogen injection rates in the feedwater compared to the recirculation piping. The second internals IGSCC mitigation technique, noble metal chemical application (NMCA), involves the continuous injection of a small amount of hydrogen to give a hydrogen to oxygen molar ratio >2 plus an occasional batch injection of noble metal compounds that act as catalysts for the various recombination reactions.
• To demonstrate that either HWC-M or NMCA provides IGSCC mitigation of BWR internals.
" To demonstrate that inspection relief is justified for BWR internals at plants that have effectively implemented HWC-M or NMCA through the use of crack growth rate factors of improvement FOIs).
One of the major problems in demonstrating the effectiveness of HWC-M or NMCA inside the reactor vessel is the difficulty of measuring the electrochemical driving force for IGSCC, i.e., the corrosion potential/electrochemical corrosion potential (ECP), of the various reactor internal components. Many plants do not have direct ECP measurements available at pertinent locations such as the lower plenum. Even those plants that do have direct measurements
available recognize that such local measurements may not be representative of all potentially susceptible component surfaces. Therefore, it was desirable to develop valid supplementary techniques that do not depend exclusively on direct measurement of the ECP at specific locations to reliably demonstrate HWC effectiveness.
To accomplish this objective, an approach was developed that can be applied in the absence of direct ECP measurements or as a supplement to direct ECP measurements. For example, ECPs can be calculated using verified computer models, (e.g., the BWRVIP radiolysis/ECP model) that can be directly correlated with measurements of other plant "secondary" parameters, (e.g., oxygen, main steam line radiation levels, etc.) and data from "sister" plants.
Results Based on the crack growth modeling and radiolysis results, a vessel internals inspection program can be developed based on FOIs for plants that have implemented either HWC-M or NMCA. The FOI calculated for each internal component based on crack growth modeling results would be applied to revise the internals inspection interval established in the various BWRVIP inspection and evaluation (I&E) documents. At a later date, the BWRVIP will propose revised inspection intervals for vessel internals for plants that have implemented either HWC-M or NMCA.
EPRI Perspective The systematic approach described in this study can be used to verify mitigation of IGSCC of reactor internals with either HWC-M or NMCA. Once IGSCC verification is obtained by using parameters such as ECPs calculated from verified computer models, measurements of other plant secondary parameters, electrochemical and chemical measurements obtained from "sister" plants, etc., the FOI approach can be applied to the current inspection criteria to provide a reduction in inspection frequency. This will lead to significant inspection cost reductions and person-Rem savings with no impact on plant reliability or safety.
Interest Categories Piping, reactor, vessel and internals Licensing and safety assessment
Key Words BWR Intergranular Stress Corrosion Cracking Reactor internals Inspection relief Hydrogen Water Chemistry Noble Metal Chemical Application
BWR Vessel and Internals Project
Technical Basis for Inspection Relief for BWR Internal Components with Hydrogen Injection (BWRVIP-62NP)
TR-108705NP Research Project B401
Final Report, February 2000
Structural Integrity Associates 6615 Almaden Expressway, Suite 24 San Jose, CA 95118-1557
GE Nuclear Energy 175 Curtner Avenue San Jose, CA 95125
EPRI 3412 Hillview Avenue Palo Alto, CA 94304
BOILING WATER REACTOR VESSEL & INTERNALS PROJECT and
3412 Hillview Ave.
Palo Alto, California 94304
DISCLAIMER OF WARRANTIES AND LIMITATION OF LIABILITIES
This report was prepared by the organization(s) named below as an account of work sponsored or cosponsored by the BWR Vessel and Internals.Project (BWRVIP) and EPRI, Inc. Neither BWRVIP, EPRI, any member of EPRI, any cosponsor, the organization(s) named below, nor any person acting on behalf of any of them:
(a) makes any warranty or representation whatsoever, express or implied, (I) with respect to the use of any information, apparatus, method, process or similar item disclosed in this report including merhantability and fitness for a particular purpose, or (ii) that such use does not infringe on or interfere with privately owned rights, including any party's intellectual property, or (iii) that this report is suitable to any particular user's circumstance, or
(b) assumes any responsibility for any damages or other liability whatsoever (including any consequential damages, even if BWRVIP, EPRI or any EPRI representative has been advised of the possibility of such damages) resulting from your selection or use of this report or an information, apparatus, method, process or similar item disclosed in this report
Organization(s) that prepared this report:
STRUCTURAL INTEGRITY ASSOCIATES GE NUCLEAR ENERGY EPRI
Requests for copies of this report should be directed to the BWRVIP Program Manager, 3412 Hillview Avenue, Palo Alto, CA, 94304, (650)-855-2340.
Boiling water reactor (BWR) availability has been negatively impacted by the intergranular
stress corrosion cracking (IGSCC) of austenitic stainless steel piping and, more recently, reactor
internal components. As mandated by Nuclear Regulatory Commission (NRC), regular
inspection is necessary for BWR piping to provide adequate assurance of structural integrity of
affected piping systems. Similar inspections may be required for reactor internal components.
However, due to the difficulty and expense of reactor internals inspections, it is clearly desirable
to demonstrate that fewer inspections are necessary when suitable reactor internals IGSCC
mitigation steps are taken.
The NRC has agreed that the environmental IGSCC mitigation technique, hydrogen water
chemistry (HWC) combined with lower water conductivity, provides a basis for inspection relief
for BWR recirculation piping (W. Sheron, NRC letter to R. A. Pinelli, BWROG, "Safety
Evaluation of Topical Report," NEDE-31951P, dated January 1995). Since the NRC established
inspection relief criteria for recirculation piping with HWC, the HWC process has been
developed along two parallel paths for mitigation of reactor internals IGSCC. The first qualified
HWC technique for reactor internals involves higher hydrogen injection rates than would
typically be used to protect recirculation piping. This process is referred as moderate HWC
(HWC-M) and results in sufficient hydrogen addition to lower ECPs to protective levels in the
lower plenum. The second equally protective technique involves the continuous injection of a
small amount of hydrogen to give a hydrogen to oxygen molar ratio >2 in the single phase liquid
region plus an occasional batch injection of catalytic noble metal compounds. This second
process is referred to as noble metal chemical application (NMCA), formally known as noble
metal chemical addition, and is also known by the GE trademark NobleChemTM. Since both
processes can protect BWR internals from environmental assisted cracking degradation, the
effective implementation of either HW